Abstract
Weyl semimetals provide the realization of Weyl fermions in solidstate physics. Among all the physical phenomena that are enabled by Weyl semimetals, the chiral anomaly is the most unusual one. Here, we report signatures of the chiral anomaly in the magnetotransport measurements on the first Weyl semimetal TaAs. We show negative magnetoresistance under parallel electric and magnetic fields, that is, unlike most metals whose resistivity increases under an external magnetic field, we observe that our high mobility TaAs samples become more conductive as a magnetic field is applied along the direction of the current for certain ranges of the field strength. We present systematically detailed data and careful analyses, which allow us to exclude other possible origins of the observed negative magnetoresistance. Our transport data, corroborated by photoemission measurements, firstprinciples calculations and theoretical analyses, collectively demonstrate signatures of the Weyl fermion chiral anomaly in the magnetotransport of TaAs.
Introduction
The principles of physics rest crucially on symmetries and their associated conservation laws. Over the past century, physicists have repeatedly observed the violations of apparent conservation laws in particle physics, each time leading to new insights and a refinement of our understanding of nature. One of the most interesting phenomena of this type is the breaking of a conservation law of classical physics by quantummechanical effects, a socalled anomaly in quantum field theory^{1}. Perhaps the most primitive example is the socalled chiral anomaly associated with Weyl fermions^{2,3,4,5,6}. A Weyl fermion is a massless fermion that carries a definite chirality. Due to the chiral anomaly, the chiral charge of Weyl fermions is not conserved by the full quantummechanical theory. Historically, the chiral anomaly was crucial in understanding a number of important aspects of the standard model of particle physics. The most wellknown case is the triangle anomaly associated with the decay of the neutral pion π^{0} (refs 3, 4). Despite having been discovered more than 40 years ago, it remained solely in the realm of highenergy physics.
Recently, there has been considerable progress in understanding the correspondence between highenergy and condensed matter physics, which has led to deeper knowledge of important topics in physics such as spontaneous symmetry breaking, phase transitions and renormalization. Such knowledge has, in turn, greatly helped physicists and materials scientists to better understand magnets, superconductors and other novel materials, leading to important practical device applications. Here, we present the signatures of the chiral anomaly in a lowenergy condensed matter Weyl system. In order to measure the chiral anomaly in a solidstate system, one needs to find a perturbation that couples differently to the two Weyl fermions of opposite chiralities. This is most naturally realized in a Weyl semimetal, in which the two Weyl cones are separated in momentum space. Recent theoretical and experimental advances have shown that Weyl fermions can arise in the bulk of certain novel semimetals with nontrivial topology^{7,8,9,10,11,12,13,14,15,16}. A Weyl semimetal is a bulk crystal whose lowenergy excitations satisfy the Weyl equation. Therefore, the conduction and valence bands touch at discrete points, the Weyl nodes, with a linear dispersion relation in all three momentum space directions moving away from the Weyl node. The nontrivial topological nature of a Weyl semimetal guarantees that Weyl fermions with opposite chiralities are separated in momentum space (Fig. 1a), and host a monopole and an antimonopole of Berry flux in momentum space, respectively (Fig. 1b). In this situation, parallel magnetic and electric fields can pump electrons between Weyl cones of opposite chirality that are separated in momentum space (Fig. 1a). This process violates the conservation of the the chiral charge, meaning that the number of particles of left and right chirality are not separately conserved^{5,17,18,19,20,21,22,23,24,25,26}, giving rise to an analogue of the chiral anomaly in a condensed matter system. Apart from this elegant analogy and correspondence between condensed matter and highenergy physics, the chiral anomaly also serves as a crucial transport signature for Weyl fermions in a Weyl semimetal phase. Furthermore, theoretical studies have recently suggested that it has potential applications^{27}.
In this paper, we perform magnetotransport experiments on the Weyl semimetal TaAs^{12,13,14,16}. We observe a negative longitudinal magnetoresistance (LMR) in the presence of parallel magnetic and electric fields, which is indicative of the chiral anomaly due to Weyl fermions. On the other hand, due to the complicated nature of the magnetoresistence^{28,29,30,31,32,33,34,35,36,37,38}, an unambiguous demonstration of the chiral anomaly remains lacking despite the volume of works reporting negative LMR^{39,40,41,42,43,44}. Our data and careful analyses, which go beyond a simple observation of a negative LMR, allow us to systematically exclude other possible origins for the observed negative LMR. These data strongly support the chiral anomaly due to Weyl fermions in TaAs. Our studies demonstrate a lowenergy platform where the fundamental physics of Weyl fermions and quantum anomalies can be studied in a piece of solid metal^{17,18,19,20,21,22,23,24,25,26,27}.
Results
ARPES band structure
We start by presenting the key aspects of the bulk band structure of TaAs both in theory and in experiment. According to our firstprinciples calculation^{13,14}, in total there are 24 bulk Weyl cones. We denote the 8 Weyl nodes that are located on the as W1 and the other 16 nodes that are away from this plane as W2 (Fig. 1c). There is a 13 meV offset between the energies of the W1 and W2 Weyl nodes (Fig. 1e). The pockets that arise from the Weyl fermions are shown in blue in Fig. 1d. Apart from the Weyl cones, there are additional (nonWeyl) holelike bands crossing the Fermi level shown by the red ringshaped contours in Fig. 1d.
We independently study the bulk electronic structure via angleresolved photoemission spectroscopy (ARPES). This is important because relying entirely on numerical band structure calculations is not conclusive. Particularly, numerical band calculations have little power in predicting the position of the chemical potential of real samples, which is crucial for transport experiments. Figure 1f shows an E−k_{} dispersion map that cuts across the two nearby W2 Weyl cones. The dispersion map reveals two linearly dispersive bands. The kspace distance between the two crossing points is about 0.08 Å^{−1}, consistent with the calculated results. More importantly, our ARPES measurement shows that the native chemical potential of the samples is very close to the energy of the W2 Weyl nodes. Our data also reveals the W1 Weyl cones. As shown in Fig. 1g, the energy of the W1 Weyl node is below that of the W2 Weyl node (Fig. 1f), which is consistent with band calculation results. Systematic ARPES data can be found in the Supplementary Fig. 1 and Supplementary Note 1. We also observe the trivial hole bands in ARPES. The essential observations are listed as follows. There are three types of bands at the Fermi level, the W1 and W2 Weyl nodes and a trivial holelike band. The native chemical potential is close to the energy of the W2 Weyl nodes, which is 13 meV higher than that of the W1 Weyl nodes. Therefore, the W1 Weyl cones form electronlike pockets, the trivial holelike bands form holelike pockets, and the W2 Weyl cones have lowcarrier concentration, which can be electron or holelike depending on the specific position of the native chemical potential with respect to the W2 Weyl node in each sample batch.
Quantum oscillation data
We have performed magnetotransport measurements on our TaAs samples, in order to probe the band structure at the Fermi level (Supplementary Fig. 2 and Supplementary Note 2). Our Hall data indeed reveal a coexistence of electron and hole carriers. We obtained critical band parameters, such as Fermi wavevector, Fermi velocity, chemical potential, carrier mobilities and so on, from the Shubnikov deHaas (SdH) oscillation data. All band parameters obtained from the SdH oscillations are consistent with firstprinciples calculation and ARPES results. Most importantly, this enables us to determine the position of the chemical potential with respect to the Weyl nodes, as shown in Fig. 2i. We name the samples by a letter (a or c) followed by a number (1–5). The letter ‘a’ or ‘c’ means that the electrical current is along the crystallographic a or caxes. The number ‘1–5’ refers to a sequence of the samples’ chemical potential with respect to the energy of the W2 Weyl node from below the node to above the node (Fig. 2i). We also provide the Fermi energy of the TaAs samples determined by different approaches in Supplementary Note 3 and Supplementary Table 1.
Longitudinal magnetoresistance
We now present our LMR data, without a prebiased assumption of their origin. Figure 2a–e show the LMR data of five different batches of samples. The LMR data show three main features as a function of the magnetic field, as schematically drawn in Fig. 2f. At very small fields close to B=0, we observe a sharp increase of the LMR. Following the sharp increase, the LMR is found to decrease in an intermediate B field range. This is the negative LMR. While further increasing the B field, the LMR starts to increase again. We note that because features I and II likely have independent origins, the LMR is not necessarily absolutely negative (we do, however, observe absolute negative LMR in samples c2 and c4). Hence, more precisely, we speak of negative LMR in this paper, if the resistivity decreases with an increasing B field. In addition to these general features, we observe other more sampledependent features: for sample c4, our data show clear quantum oscillations at a quite wide B field range of 0.5 T≤B≤8 T. For other samples, the quantum oscillations are much weaker but they are still visible. For sample a5, the LMR increases monotonically as a function of the B field. No negative LMR is observed.
We study the systematic dependence of the LMR on different parameters, including temperature, the angle between the and fields, and the direction of the current with respect to the crystallographic axis. The temperaturedependent data are shown in Fig. 3a for sample a1. Most notably, the negative LMR (feature II) shows a strong temperature dependence. At higher temperatures, for example, T≥50 K, the negative LMR vanishes. The dependence on the angle between the and fields are shown in Fig. 3b–e. Our data show that the negative MR exhibits a very strong angular dependence. It becomes quickly suppressed as one varies the direction of the magnetic field away from that of the electric field. The dependence on the direction of the current with respect to the crystallographic direction is presented in Fig. 2. The measurements were performed with current along the crystallographic a axis for samples a1, a3 and a5, and with current along the c axis for samples c2 and c4. In both cases, the negative LMR is observed except for sample a5, whose chemical potential is far away from the energy of the Weyl nodes (Fig. 2i).
Origins of the negative LMR
We now use these observations to understand the origin of the negative LMR. First, it is wellknown that a negative LMR can arise in magnetic materials^{28}. This obviously does not apply to our nonmagnetic TaAs samples. The second possible origin is more classical due to geometry or size effects of the samples, such as the currentjetting effect^{29,30}. These geometrical MR effects are also not consistent with our data, because they do not vanish quickly as one raises temperature^{30}, and furthermore we have carefully shaped our samples to exclude the geometrical effects (Supplementary Fig. 3 and Supplementary Note 4). Third, we observe the negative LMR with current flowing both along the crystallographic a and caxes. We note that TaAs has a tetragonal lattice. Hence the a and caxes represent the largest anisotropy that the system could offer. The fact that the negative LMR is observed along both a and caxes proves that anisotropies in the system cannot explain our data^{32}. Fourth, in the quantum limit, negative LMR can arise from the chiral, quasi onedimensional character of the Landau levels that are formed by the band structure under magnetic fields. Essentially, it was predicted^{31,33} that a negative LMR can arise in any 3D metal irrespective of its band structure if the sample is in the ultraquantum limit, which means that one has (ω is the cyclotron frequency and is the transport life time) and that the chemical potential only crosses the lowest Landau level (the Landau level index N=0, see Supplementary Fig. 4). This has been observed in doped semiconductor samples^{35}. We have carefully checked whether our negative LMR is due to this mechanism. Particularly, one needs to be careful about the trivial holelike bands in TaAs, because if they were in the ultraquantum limit then it would have been entirely possible that the observed negative LMR were due to these trivial bands, rather than due to Weyl fermions in our samples. We note that the negative LMR are observed at small magnetic fields (for example, 0.1 T≤B≤0.5 T for sample a1). We have checked the and the Landau level index N of our samples quantitatively (Supplementary Table 2), and our results show that all samples are always in the semiclassical limit at the small magnetic fields where the negative LMR are observed. Therefore, our data are inconsistent with this origin^{31,33}. Fifth, a recent theoretical work has predicted a linear Bdependent magnetoconductivity in small fields^{45}. However, this is also inconsistent with our data because predicted linear Bdependent magnetoconductivity requires the system to lie in the ultraquantum limit. That is, only the lowest Landau band crosses the Fermi level, which is clearly not the case for our systems under study. Finally, in the semiclassical limit, nonzero LMR can arise from finite Berry curvature, as follows from the semiclassical equations of motion. Having excluded all other possibilities, we are led to conclude that our observed negative LMR must have this origin. However, as suggested in ref. 36 in addition to nonzero Berry curvature, an approximately conserved chiral charge density with long relaxation time—as found in Dirac and Weyl semimetals—is required to yield a negative LMR. The observed negative LMR is most likely to be attributed to Weyl nodes, in accordance with the theoretical analysis of (refs 24, 26 and 36). To confirm this picture independent of the assumption of effective lowenergy Weyl Hamiltonians, we have studied the contribution of Berry curvature from each band carefully in a firstprinciplesderived model for TaAs (see Fig. 4c,d and Supplementary Fig. 5 and Supplementary Note 5). Our results show that in our TaAs system the Berry curvature almost entirely arises from the Weyl cones.
The chiral anomaly
With such a conclusion, we are entitled to fit our LMR data with a semiclassical magnetoconductance formula that includes the contribution from Weyl nodes due to their Berry curvature. Specifically, we use the following equation.
All coefficients are positive. The first term σ^{chiral}=C_{W}B^{2} is due to the Weyl fermions and will lead to a B^{2}dependent negative LMR. This term was systematically studied by transport theories in refs 24, 26. The chiral coefficient is (refs 24, 26), where g(E_{F}) is the density of states at the Fermi level, is the axial charge relaxation time and the additional factor of 8 is because we have 8 pairs of W2 Weyl nodes. All remaining terms contribute to positive LMR in the semiclassical regime. The C_{WAL} term arises from the 3D weak antilocalization (WAL) effect of the Weyl cones, which accounts for the initial steep uprise of the LMR at small magnetic fields. The 3D WAL is known to have a−B^{2} dependence near zero field and dependence at higher fields^{46}. So we include a critical field B_{c} that characterizes a crossover. For the four samples a1, c2, a3, c4, the increase of the LMR at small magnetic fields are 230, 5, 156 and 47% compared to the zerofield resistance. Particularly, the increase for samples a1 and a3 is larger than 100%, which is usually not expected from the WAL scenario. On the other hand, we do notice that the increase is quite sample dependent, and that a similarly large increase (∼100%) of the magnetoresistance has also been reported in a concurrent transport work on TaAs^{40}. In this work, we fit this initial uprise of the LMR by the WAL effect, but the anomalously large increase in samples a1, a3 and also in ref. 40 remains an theoretically open question that needs further investigation, which does not affect our main conclusion, that is, signatures of the chiral anomaly. Finally, the σ_{0} term is the positive LMR that arises from the Drude conductivity of conventional charge carriers present in TaAs. In parallel fields, the Lorentz force is zero so the Drude conductivity is a constant. More systematic details regarding the fitting are presented in Supplementary Fig. 6 and Supplementary Note 6.
The fitting results are shown by the green curves in Figs 2a–e and 3a,b. It can be seen that the fitting works well for the small B field region which includes the negative LMR. This is reasonable because the fitting formula is derived in the semiclassical limit. The angle dependence of the chiral coefficient C_{W} is shown in Fig. 4b for sample a3, which demonstrates that C_{W} is only significant in the presence of parallel electric and magnetic fields. The sharp angular dependence is an open theoretical problem. More importantly, we study the chemicalpotential dependence of the LMR data. Our fitting captures quantitatively the relative size of the lowfield positive LMR and the higherfield negative LMR as a function of chemical potential. We plot this ratio as a dimensionless quantity in Fig. 4a. We find that despite the simple form of the fitting formula, the different measurement geometries for the different samples, the presence of large quantum oscillations in sample c4 and large differences in the absolute resistivities of different samples, the chiral anomaly ratio scales as . It is remarkable that this fitting result matches the simplest theoretical model for a Weyl point, where the Berry curvature . We emphasize that this provides powerful evidence that the negative LMR is due to the Weyl fermions. Note that the specific expression of the chiral coefficient, , is a result of the linear dispersion and the specific Berry curvature distribution of the Weyl cones (see Fig. 1b). Especially, at the energy of the W2 Weyl nodes, the trivial hole bands do not have any singularity. Thus if the negative LMR arose from the hole bands, then the chiral coefficient C_{W} would not have increased markedly as the chemical potential approaches the energy of the W2 Weyl nodes (Fig. 4a). Therefore, the obtained dependence of the chiral coefficient (Fig. 4a) provides a unique demonstration that our negative LMR is due to the Weyl fermions, because the dependence reveals the details of the band dispersion and Berry curvature distribution of the Weyl cones, not just the fact that the bands have some nonzero Berry curvature. We use the above data and analyses to further exclude the possibility of negative LMR due to weak localization arising from the intervalley scattering. Our data is not due to the weak localization for the following reasons: First, weak localization does not have a strong E_{F} dependence, let alone the marked dependence observed in our data. Second, it has been theoretically shown that the magnetoconductivity without the chiral anomaly is always monotonic, even though the intervalley scattering can induce a negative LMR arising from the weak localization^{46}. This is not consistent with our data, which means that, without the chiral anomaly, only weak localization/antilocalization cannot explain our data.
Up to here, we have demonstrated that the negative LMR arises from the nonzero Berry curvature of the Weyl fermions in our TaAs samples. We now establish the connection between our data and the chiral anomaly, the nonconservation of the electron quasiparticle number of the Weyl cones with a given chirality. In a real Weyl semimetal sample, this can be understood by two crucial components, the axial chargepumping effect and the axial charge relaxation, as schematically shown in Fig. 4f. The chargepumping effect means that a nonzero E·B can pump charges from one Weyl cone to the other, leading to an imbalance of the quasiparticle number of the Weyl cones with the opposite chiralities. This effect is wellestablished to occur between Weyl nodes of different chiral charge^{24,26,36}, which are monopoles of Berry field strength in momentum space. We have directly shown the nontrivial Berry curvature monopoles associated with the Weyl fermions via our LMR transport data. The axial charge pumping creates an outofequilibrium quasiparticle distribution between the Weyl cones with opposite chiralities. To form a steady state, it is counteracted by the relaxation of the axial charge disproportionation through scattering between the Weyl nodes. The relaxation is characterized by a time scale, the axial charge relaxation time . From our negative LMR data, we directly obtain the axial charge relaxation time (Fig. 4e). The nonzero axial charge relaxation time not only directly demonstrates the axial charge relaxation, but also confirms the existence of the axial charge pumping because these two are directly coupled, which means that one cannot exist alone if the other is absent.
We can directly obtain the axial charge relaxation time , which serves as the critical physical quantity that characterizes the chiral anomaly, from the chiral coefficient C_{W} using the relationship (refs 24, 26). In Fig. 3a, we present fitting results as a function of temperature for sample s1. We use the fitting coefficients C_{W} to obtain the axial charge relaxation time as a function of temperature, presented in Fig. 4e. We find that the rapidly decays to zero with increasing temperature. This decay of corresponds to the decay of the negative LMR with increasing temperature in the raw data and is expected because scattering typically increases with temperature. We obtain an axial charge relaxation time =5.96 × 10^{−11} s for sample a1 at T=2 K (Fig. 4e). Note that this is associated with the W2 Weyl cones because the Fermi level is very close to the W2 nodes. On the other hand, it is difficult to obtain the transport life time of the W2 Weyl cones because the density of states at the Fermi level is dominated by contributions from the W1 Weyl cones and the trivial hole bands (Fig. 1d). Therefore, we estimate the quasiparticle life time associated with the W2 Weyl cones via ≃ħ/E_{F}=7.04 × 10^{−13} s for sample a1. We see that the axial charge relaxation time is much longer than the quasiparticle life time . The imbalance of population due to the axial charge pumping can be also estimated by the uncertainty principle Δμ=ħ/≃0.011 meV. At E_{F}=−1.5 meV, the density of states per W2 Weyl cone is g(E_{F})=1.6 × 10^{16} states/(eV cm^{−3}). Therefore, we estimate the chiral charge, the nonconservation of the quasiparticle number of the Weyl cone with a given chirality, to be Δμ × g(E_{F})=1.6 × 10^{14}. This directly characterizes the chiral anomaly in our Weyl semimetal TaAs sample.
Discussion
We emphasize the critical logical sequences that are key to our demonstration. Unlike previous studies, we do not assume that the negative LMR arises from the chiral anomaly^{40,41,42,43,44}. To demonstrate the chiral anomaly, it is critically important to consider all possible origins for a negative LMR and to discuss how one can distinguish each of the other origins from the chiral anomaly. We first excluded the geometry and spin(magnetic) effects. Then we show that our observed LMR is not in the quantum (large B field) limit, in which the Fermi energy crosses only the lowest Landau level. This is important because the LMR in the quantum (large B field) limit can be negative or positive depending on specific scenarios, such as the band dispersion and nature of the impurities^{31,33,34}. In fact, it is even theoretically shown that the Weyl cones that respect timereversal symmetry can contribute a positive (not a negative) LMR in the quantum limit if the field dependence of the scattering time and Fermi velocity of the Landau bands is fully respected^{34}. Therefore, observing a negative LMR in the largefield quantum limit may not be a compelling signature of Weyl fermions. In the semiclassical (small B field) limit, after excluding the geometry and magnetic effects, one can avoid ambiguities in the physical interpretation since a negative LMR can only arise from a nonzero Berry curvature^{24,26,36,37}. In fact, it has been shown that the LMR from a band with zero Berry curvature will always be positive^{37}. However, we emphasize that, at a qualitative level, the negative LMR in the semiclassical limit is only a signature of the Berry curvature but it is not unique to Weyl fermions. In order to uniquely attribute the negative LMR to Weyl fermions, we discovered here that it is crucial to obtain comprehensive information about the band structure. Specifically, first we have shown that the Berry curvature in our TaAs is dominated by the Weyl cones. Second, the chiral coefficient has a dependence. These two pieces of evidence, together with the full systematics of the data sets uniquely presented here, provides strong signatures of the chiral anomaly of Weyl fermions.
Methods
Sample growth and electrical transport
Highquality single crystals of TaAs were grown by the standard chemical vapour transport method as described in ref. 47. TaAs crystals were structurally characterized by powder Xray diffraction to confirm bulk quality, and to determine (001) crystal face. A small portion of the obtained samples were ground into fine powders for Xray diffraction measurements on Rigaku MiniFlex 600 with Cu K_{α} (40 kV, 15 mA; λ=0.15405, nm) at room temperature, and then refined by a Rietica Rietveld program. Magnetotransport measurements were performed using a Quantum Design Physical Property Measurement System. Highfield electrical transport measurements were carried out using a pulsed magnet of 50 ms in Wuhan National High Magnetic Field Center. All the measurements were carried out from −9 to 9 T or −56 to 56 T.
Angleresolved photoemission spectroscopy
The soft Xray ARPES (SXARPES) measurements were performed at the ADRESS Beamline at the Swiss Light Source in the Paul Scherrer Institut in Villigen, Switzerland using photon energies ranging from 300 to 1,000 eV (ref. 48). The sample was cooled down to 12 K to quench the electron–phonon interaction effects reducing the kresolved spectral fraction. The energy and angle resolution was better than 80 meV and 0.07°, respectively. Vacuum ultraviolet ARPES measurements were performed at beamlines 4.0.3, 10.0.1 and 12.0.1 of the Advanced Light Source at the Lawrence Berkeley National Laboratory in Berkeley, California, USA, Beamline 5–4 of the Stanford Synchrotron Radiation Light source at the Stanford Linear Accelerator Center in Palo Alto, California, USA and Beamline I05 of the Diamond Light Source in Didcot, UK, with the photon energy ranging from 15 to 100 eV. The energy and momentum resolution was better than 30 meV and 1% of the surface Brillouin zone.
Theoretical calculations
Firstprinciples calculations were performed by the OPENMX code within the framework of the generalized gradient approximation of densityfunctional theory^{49}. Experimental lattice parameters were used^{47}, and the details for the computations can be found in our previous work in ref. 13. A realspace tightbinding Hamiltonian was obtained by constructing symmetryrespecting Wannier functions for the As p and Ta d orbitals without performing the procedure for maximizing localization, similar for calculations done for topological insulators^{50,51}.
Additional information
How to cite this article: Zhang, C.L. et al. Signatures of the Adler–Bell–Jackiw chiral anomaly in a Weyl fermion semimetal. Nat. Commun. 7:10735 doi: 10.1038/ncomms10735 (2016).
References
Bertlmann, R. A. Anomalies in Quantum Field Theory International Series of Monographs on Physics (2011).
Weyl, H. Elektron und gravitation. I. Z. Phys. 56, 330–352 (1929).
Adler, S. Axialvector vertex in spinor electrodynamics. Phys. Rev. 177, 2426–2438 (1969).
Bell, J. S. & Jackiw, R. A PCAC puzzle: π^{0}→γγ in the σmodel. Il. Nuovo. Cimento. A 60, 47–61 (1969).
Nielsen, H. B. & Ninomiya, M. The AdlerBellJackiw anomaly and Weyl fermions in a crystal. Phys. Lett. B 130, 389–396 (1983).
Volovik, G. E. The Universe in a Helium Droplet Clarendon Press (2003).
Balents, L. Weyl electrons kiss. Physics 4, 36 (2011).
Wan, X. G., Turner, A. M., Vishwanath, A. & Savrasov, S. Y. Topological semimetal and fermiarc surface states in the electronic structure of pyrochlore iridates. Phys. Rev. B 83, 205101 (2011).
Hasan, M. Z., Xu, S.Y. & Neupane, M. in Topological Insulators: Fundamentals and Perspectives eds Ortmann F., Roche S., Valenzuela S. O. John Wiley & Sons (2015).
Turner, A. M. & Vishwanath, A. in Topological Insulators eds Franz M., Molenkamp L. Elsevier (2013).
Murakami, S. Phase transition between the quantum spin Hall and insulator phases in 3D: emergence of a topological gapless phase. New. J. Phys. 9, 356 (2007).
Xu, S.Y. et al. Discovery of a Weyl Fermion semimetal and topological Fermi arcs. Science 349, 613–617 (2015).
Huang, S. M. et al. A Weyl Fermion semimetal with surface Fermi arcs in the transition metal monopnictide TaAs class. Nat. Commun. 6, 7373 (2015).
Weng, H. et al. Weyl semimetal phase in noncentrosymmetric transition metal monophosphides. Phys. Rev. X 5, 011029 (2015).
Lu, L. et al. Experimental observation of Weyl points. Science 349, 622–624 (2015).
Lv, B. Q. et al. Experimental discovery of Weyl semimetal TaAs. Phys. Rev. X 5, 031013 (2015).
Duval, C., Horvath, Z., Horvathy, P. A., Martina, L. & Stichel, P. C. Berry phase correction to electron density in solids and “exotic” dynamics. Mod. Phys. Lett. B 20, 373 (2006).
Fukushima, K., Kharzeev, D. E. & Warringa, H. J. Chiral magnetic effect. Phys. Rev. D 78, 074033 (2008).
Zyuzin, A. A. & Burkov, A. A. Topological response in Weyl semimetals and the chiral anomaly. Phys. Rev. B 86, 115133 (2012).
Aji, V. AdlerBellJackiw anomaly in Weyl semimetals: application to pyrochlore iridates. Phys. Rev. B 85, 241101 (2012).
Zyuzin, A. A., Wu, S. & Burkov, A. A. Weyl semimetal with broken time reversal and inversion symmetries. Phys. Rev. B 85, 165110 (2012).
Grushin, A. G. Consequence of a condensed matter realization of Lorentzviolating QED in Weyl semimetals. Phys. Rev. D 86, 045001 (2012).
Hosur, P. & Qi, X.L. Recent developments in Weyl semimetals. Comptes. Rendus. Physique. 14, 857–870 (2013).
Son, D. T. & Spivak, B. Z. Chiral anomaly and classical negative magnetoresistance of Weyl metals. Phys.Rev. B 88, 104412 (2013).
Jho, Y.S. & Kim, K.S. Interplay between interaction and chiral anomaly: anisotropy in the electrical resistivity of interacting Weyl metals. Phys. Rev. B 87, 205133 (2013).
Burkov, A. A. Chiral anomaly and diffusive magnetotransport in Weyl metals. Phys. Rev. Lett. 113, 247203 (2014).
Parameswaran, S. A., Grover, T., Abanin, D. A., Pesin, D. A. & Vishwanath, A. Probing the chiral anomaly with nonlocal transport in threedimensional topological semimetals. Phys. Rev. X 4, 031035 (2014).
Ritchie, L. et al. Magnetic, structural, and transport properties of the Heusler alloys Co2MnSi and NiMnSb. Phys. Rev. B 68, 104430 (2003).
Pippard, A. B. Magnetoresistance in Metals Cambridge University Press (1989).
Hu, J., Rosenbaum, T. F. & Betts, J. B. Current jets, disorder, and linear magnetoresistance in the silver chalcogenides. Phys. Rev. Lett. 95, 186603 (2005).
Argyres, P. N. & Adams, E. N. Longitudinal magnetoresistance in the quantum limit. Phys. Rev. 104, 900–908 (1956).
Kikugawa, et al. Realization of the axial anomaly in a quasitwodimensional metal. Preprint at http://arxiv.org/abs/1412.5168 (2014).
Goswami, P., Pixley, J. H. & Das Sarma, S. Axial anomaly and longitudinal magnetoresistance of a generic three dimensional metal. Phys. Rev. B 92, 075205 (2015).
Lu, H.Z., Zhang, S.B. & Shen, S.Q. Highfield magnetoconductivity of topological semimetals with shortrange potential. Phys. Rev. B 92, 045203 (2015).
Sugihara, K., Tokumoto, M., Yamanouchi, C. & Yoshihiro, K. Longitudinal magnetoresistance of nInSb in the quantum limit. J. Phys. Soc. Jpn 41, 109–115 (1976).
Burkov, A. A. Negative longitudinal magnetoresistance in Dirac and Weyl metals. Phys. Rev. B 91, 245157 (2015).
Pal, H. K. & Maslov, D. L. Necessary and sufficient condition for longitudinal magnetoresistance. Phys. Rev. B 81, 214438 (2010).
Spivak, B. Z. & Andreev, A. V. Magnetotransport phenomena related to the chiral anomaly in Weyl semimetals. Preprint at http://arxiv/abs/1510.01817 (2015).
Kim, H.J. et al. Dirac versus Weyl Fermions in topological insulators: AdlerBellJackiw anomaly in transport phenomena. Phys. Rev. Lett. 111, 246603 (2013).
Huang, X. et al. Observation of the chiral anomaly induced negative magnetoresistance in 3D Weyl semimetal TaAs. Phys. Rev. X 5, 031023 (2015).
Zhang, C. et al. Observation of the AdlerBellJackiw chiral anomaly in a Weyl semimetal. Preprint at http://arxiv.org/abs/1503.02630 (2015).
Xiong, J. et al. Sinature of the chiral anomaly in a Dirac semimetal: a current plume steered by a magnetic field. Preprint at http://arxiv.org/abs/1503.08179 (2015).
Zhang, C. et al. Detection of chiral anomaly and valley transport in Dirac semimetals. Preprint at http://arxiv.org/abs/1504.07698 (2015).
Shekhar, C. et al. Large and unsaturated negative magnetoresistance induced by the chiral anomaly in the Weyl semimetal TaP. Preprint at http://arxiv.org/abs/1506.06577 (2015).
Zhang, S.B., Lu, H.Z. & Shen, S.Q. Chiral anomaly and linear magnetoconductivity in a topological Weyl semimetal. Preprint at http://arxiv.org/abs/1509.02001 (2015).
Lu, H.Z. & Shen, S.Q. Weak antilocalization and localization in disordered and interacting Weyl semimetals. Phys. Rev. B 92, 035203 (2015).
Murray, J. J. et al. Phase relationships and thermodynamics of refractory metal pnictides: the metalrich tantalum arsenides. J. Less Common Met. 46, 311–320 (1976).
Strocov, V. N. et al. oftXray ARPES facility at the ADRESS beamline of the SLS: concepts, technical realisation and scientific applications. J. Synchrotron Rad. 21, 32–44 (2014).
Perdew, J. P., Burke, K. & Ernzerhof, M. Generalized gradient approximation made simple. Phys. Rev. Lett. 77, 3865–3868 (1996).
Hasan, M. Z. & Kane, C. L. Topological insulators. Rev. Mod. Phys. 82, 3045–3067 (2010).
Weng, H., Ozaki, T. & Terakura, K. Revisiting magnetic coupling in transitionmetalbenzene complexes with maximally localized Wannier functions. Phys. Rev. B 79, 235118 (2009).
Acknowledgements
M.Z.H., S.Y.X. and I.B. thank I. Klebanov, A. Polyakov and H. Verlinde for theoretical discussions. T.N. thanks A.G. Grushin for discussions. S.J. thanks J. Xiong and F. Wang for valuable discussions, and C.L.Z. and Z.Y. thank Y. Li and J. Feng for using instruments in their groups. The work at Princeton and Princetonled synchrotronbased measurements were supported by Gordon and Betty Moore Foundation through Grant GBMF4547 (Hasan). S.J. was supported by the National Basic Research Program of China (Grant Nos. 2013CB921901 and 2014CB239302) and by the Opening Project of Wuhan National High Magnetic Field Center (Grant No.PHMFF2015001), Huazhong University of Science and Technology. C.Z. was supported by the National Science Foundation of China (Grant No.11374020). H.Z.L. acknowledges the Singapore National Research Foundation for the support under NRF Award No. NRFNRFF201303. S.Q.S. was supported by the Research Grant Council, University Grants Committee, Hong Kong under Grant No. 17303714. M.N. was supported by the startup funds from University of Central Florida and Los Alamos National Laboratory Laboratory Directed Research & Development (LDRD) program. H.L. was supported by the Natural Science Foundation of China under Grant No. 11574127. We gratefully acknowledge J.D. Denlinger, S.K. Mo, A.V. Fedorov, M. Hashimoto, M. Hoesch, T. Kim and V.N. Strocov for their beamline assistance at the Advanced Light Source, the Stanford Synchrotron Radiation Lightsource, the Diamond Light Source and the Swiss Light Source. Visits to Princeton University by S.M.H., G.C., T.R.C and H.L. were partially funded by the U.S. Department of Energy (DOE), Office of Science, Basic Energy Sciences (BES) under the funding number DEFG0205ER46200.
Author information
Affiliations
Contributions
C.L.Z., performed the electrical transport experiments with help from Z.Y., Z.L., B.T., J.W., C.Z. and S.J.; S.Y.X., I.B., G.B. conducted the ARPES experiments with assistance from N.A., M.N., D.S.S., H.Z. and M.Z.H.; C.L.Z., Z.Y. and S.J. grew the singlecrystal samples; C.C.L., S.M.H., T.R.C., G.C., C.H.H., H.T.J. and H.L. performed firstprinciples band structure calculations; H.Z.L., S.Q.S. and T.N. did theoretical analyses; H.Z.L. and S.Q.S. proposed the fitting formula for the weak antilocalization. I.B. performed the fitting to the magnetoresistance data. S.Y.X., M.Z.H. and S.J. were responsible for the overall direction, planning and integration among different research units.
Corresponding authors
Ethics declarations
Competing interests
The authors declare no competing financial interests.
Supplementary information
Supplementary Information
Supplementary Figures 16, Supplementary Tables 12, Supplementary Notes 17 and Supplementary References (PDF 1275 kb)
Rights and permissions
This work is licensed under a Creative Commons Attribution 4.0 International License. The images or other third party material in this article are included in the article’s Creative Commons license, unless indicated otherwise in the credit line; if the material is not included under the Creative Commons license, users will need to obtain permission from the license holder to reproduce the material. To view a copy of this license, visit http://creativecommons.org/licenses/by/4.0/
About this article
Cite this article
Zhang, CL., Xu, SY., Belopolski, I. et al. Signatures of the Adler–Bell–Jackiw chiral anomaly in a Weyl fermion semimetal. Nat Commun 7, 10735 (2016). https://doi.org/10.1038/ncomms10735
Received:
Accepted:
Published:
DOI: https://doi.org/10.1038/ncomms10735
Further reading

Tunable Berry curvature and transport crossover in topological Dirac semimetal KZnBi
npj Quantum Materials (2021)

Anomalous negative longitudinal magnetoresistance and violation of Ohm's law deep in the topological insulating regime in Bi$$_{1x}$$Sb$$_x$$
Scientific Reports (2021)

2D weak antilocalization in thin films of the topological semimetal Pd$$_{3}$$Bi$$_{2}$$S$$_{2}$$
Scientific Reports (2021)

Thermal chiral anomaly in the magneticfieldinduced ideal Weyl phase of Bi1−xSbx
Nature Materials (2021)

Kramers Weyl semimetals as quantum solenoids and their applications in spinorbit torque devices
Communications Physics (2021)
Comments
By submitting a comment you agree to abide by our Terms and Community Guidelines. If you find something abusive or that does not comply with our terms or guidelines please flag it as inappropriate.